## Abstract

Stabilization of the 2*H* phase of MoTe_{2} during molecular beam epitaxy (MBE) growth on graphene terminated 6*H*-SiC(0001) is highly desirable in order to take advantage of its promising properties in electronic applications. By properly adjusting the conditions, direct growth of the highly crystalline 2*H* phase of MoTe_{2} has been achieved. In such van der Waals heterostructure, the atomically-clean interface between graphene and MoTe_{2} permits the electronic coupling between the adjacent layers and the emergence of a high variety of Moiré patterns. In this paper, we investigate a single layer of 2*H*-MoTe_{2} grown on graphene by MBE and we present scanning tunneling microscopy (STM) investigations combined with density functional theory (DFT) calculations and simulations of STM images. Our results show that the STM images of the MoTe_{2}/graphene heterostructure surprisingly amplify the otherwise weak Moiré potential modulations leading to the appearance of unique higher-indexed Moiré patterns. These patterns are unusually rich with many Fourier-overtones and show a remarkable variety of different applied bias voltages, revealing the complex electronic features of the heterostructure.

### Similar content being viewed by others

## Introduction

In recent years, the progress of 2D materials growth and characterization has been significantly governed by the study of transition metal dichalcogenides (TMDs)^{1}. TMDs exhibit unique electrical and optical properties due to their tunable bandgap and the transition from an indirect bandgap in bulk to a direct bandgap in monolayer. Strong photoluminescence^{2} and large exciton binding energy^{3} make them a promising candidate for a variety of optoelectronic devices, including solar cells^{4}, photo-detectors^{5}, light-emitting diodes^{6}, and photo-transistors^{7}. However, defect-free growth and detailed structural and electronic characterization of monolayer TMDs on desired substrates are still challenging.

Compared with other TMD materials, MoTe_{2} possesses some distinct properties that make it attractive for research. Of the two phases (1*T*’ and 2*H*) that are stable at room temperature^{8,9}, the 2*H* phase displays a direct bandgap of ~1 eV, similar to that of Si, making it desirable for ambipolar field-effect transistors^{10}. Many recent studies report on the growth of MoTe_{2} on different substrates using various methods such as the Te flux controlled chemical vapor deposition (FCCVD)^{11,12,13}, chemical vapor transport (CVT)^{14,15}, chemical vapor deposition (CVD)^{16,17,18}, magnetron sputtering^{19}, and molecular beam epitaxy (MBE)^{20,21,22,23}. MBE has proven the great advantages of precise growth control under highly reproducible conditions due to slow growth rates and the deposition in an ultra-high vacuum environment at lower growth temperatures^{9}. The phase and the crystalline quality of MoTe_{2} are also closely related to the choice of the suitable substrate. Graphene is recognized as one of the most promising ones for growing high-quality MoTe_{2} because it is chemically inert with honeycomb structure, ideal for van der Waals (vdW) epitaxy and unstrained growth^{21}. However, the practical production of the desired MoTe_{2} phase encounters difficulties as a result of the very small formation energy difference between 2*H* and 1*T*’ phases in the films (~0.04 eV/MoTe_{2})^{24} and therefore requires very precise control of the growth conditions. In this context, we have previously reported MBE growth of MoTe_{2} on graphene with the desired phase and good crystallinity^{9,25}. We have found that single-layer 2*H*-MoTe_{2} films (referred to as 1*H* hereafter) grown on graphene induce the formation of Moiré patterns with various twist angles in a wide interval^{9}. This phenomenon is also influenced by the synthesis conditions such as substrate temperature, beam flux, and post-growth annealing time^{9,26}.

Moiré pattern between 2D heterostructures^{27} is very common as these systems are held together by vdW forces, which allow them to rotate relative to each other easily. These Moiré patterns have important consequences on the physical properties of the systems. A prime example is the particular electronic behavior of bilayer graphene with a small magic angle, which has opened a new area of research, the twistronics^{28,29}. As first described by Zeller et al. in detail^{30,31} and later by ref. ^{32}, Moiré patterns can be categorized according to the indices (*m**n**p**q*) based on the reciprocal lattice vectors of the constituent layers (\({\overrightarrow{G}}_{mn}\), \({\overrightarrow{G}}_{pq}^{\prime}\)). Zeller et al. treated the frequency domain of the patterns transferring the problem of a Moiré lattice to the optical analog of a beat. In hexagonal systems, the most common Moiré pattern is the one with the lowest possible (*m**n**p**q*) indices i.e., (1010) as commonly observed in several heterostructures such as graphene on graphene^{33}, graphene on hexagonal boron nitride (h-BN)^{34}, MoTe_{2} on MoS_{2}^{35} to name a few examples. Higher-indexed patterns typically have weaker potential modulation, and therefore their detection by scanning tunneling microscopy (STM) is limited. However, such higher-indexed patterns are expected to be observable around the twist angle of 30^{∘}^{36,37} because at such twist angles in hexagonal lattices, the wavelength of the dominant (1010) pattern becomes comparable to the atomic lattice, and therefore will no longer be observable, not masking anymore the higher-indexed patterns. The observation of the higher-indexed patterns is further complicated for commensurate heterostructures having finite supercells. In this case, the perfect atomic periodicity, i.e., the size of the supercell, can be larger than the Moiré periodicity, which appears beside the different Moiré patterns. While ref. ^{32} only treated the occurring frequencies of the pattern and left out the question of commensurability, Zeller et al. focused on this issue. In this context, the question arises whether or not patterns contain a quasiperiodic motif (introduced by ref. ^{36}) or a true commensurate unit cell.

In this paper, we show that unusual higher-indexed Moiré patterns together with the periodicity of commensurate supercells are observed by STM in the MoTe_{2}/graphene heterostructure around 30^{∘} rotation angles. Moreover, we observe that these Moiré patterns depend strongly on the bias voltage. In heterostructures, some features of Moiré patterns can depend on the bias voltage. This can affect the amplitude of electronic corrugation^{38}, or even contrast inversion^{39} can occur. However, here we report the unique drastic change of the Moiré periodicity with the bias voltage, indicating the presence of several higher-indexed patterns, amongst which one can selectively switch by changing the bias. This variability of the charge density is attributed to the competing contribution of Mo and Te orbitals for different bias voltages and to the strong influence of the graphene substrate, as revealed by our density functional theory (DFT) calculations. The presence of the higher-indexed Moiré makes the apparent patterns unusually rich and complex in the case of the MoTe_{2}/graphene heterostructure grown by MBE with high crystalline quality.

## Results and discussion

### STM of MoTe_{2} on graphene

The experimental analyses of STM images before and after 2*H*-MoTe_{2} grown on graphene are presented in Fig. 1.

In Fig. 1a, a large STM image of 500 × 500 nm^{2} with proper flat terraces of pristine graphene is shown together with an atomic resolution of the honeycomb structure in the inset, confirming the high crystalline quality of prepared graphene. After MoTe_{2} formation (Fig. 1b), domains of a 2*H* structure are visible along with a small fraction of exposed graphene which can still be observed, labeled as “G” on the figure. The first layer of 2*H*-MoTe_{2} (named 1*H*) covers most of the graphene surface. Small portions of a second layer (named 2*H*) form on the top of the first layer in the AB stacking order as evidenced by our previous study^{9}. The LEED pattern (inset) shows a bright diffraction ring corresponding to the 2*H* phase. The additional diffraction spots originate from graphene and SiC substrate exclusively, which confirms that only the 2*H*-MoTe_{2} phase was grown on graphene with high crystalline quality. The ring pattern is associated with a large number of micron-size crystallites of 2*H*-MoTe_{2} with random in-plane orientations around a preferential orientation that is aligned with the graphene substrate. For further detailed information on single-phase stabilization, the tunneling current density of corresponding STM images together with RHEED and LEED (at low beam energy) patterns are also provided in Supplementary Fig. 1.

The height of the 2*H* layer is measured along the black line of Fig. 1b and shown in Fig. 1g. The average height between 1*H* and graphene (~4–6 Å) is lower than the height between 1*H* and 2*H*-MoTe_{2} (~6–7 Å) from the measured height profile (see in Fig. 1h). The apparent height difference between the first and second layer of MoTe_{2} is explained by the difference in the local density of states (LDOS) of the graphene and the MoTe_{2} probed by the STM measurements at the applied bias voltage. Our DFT calculations proved that the lower LDOS on the domain of 1*H*-MoTe_{2} requires the STM tip to move closer to the sample surface by ~2 Å to maintain the same tunneling current as on graphene support.

By zooming on 40 × 40 nm^{2} of the 1*H* domain, three different periodic structures can be observed, marked as regions **(I)**, **(II)**, and **(III)** in Fig. 1c. Close-up imaging on the black squares of each region reveals Moiré patterns with surprisingly rich and complex inner textures shown in Fig. 1d–f. Figure 2 shows high-resolution STM images on a region at the interface between **(I)** and **(III)** using different sample biases. At the atomic scale, Moiré patterns can be clearly identified with supercells marked by black and green rhombuses on each region. As can already be seen here, these patterns are quite sensitive to the bias voltage. It is worth noting that previous STM studies show a dense triangular network of line defects in TMD samples grown by MBE, which are associated with mirror twin boundaries (MTBs)^{40,41,42,43,44}. However, those MTBs in the literature usually preserve their line format and do not show such a variation of the STM image with the bias voltage in sharp contrast with our Moiré patterns. Based on the periodicity of each supercell (~1.23 and ~1.85 nm respectively) in Fig. 2, this information along with theoretical lattice constants served as an input to a simple geometrical model to iterate through a large number of possible commensurate supercells as described in refs. ^{45,46}, finding the ones that match the experimental layouts. We kept here the lattice constant of the graphene substrate at a fixed value of 2.46 Å. Consequently, the possible commensurate structures are formed only at well-defined, discrete value pairs of the twist angle and MoTe_{2} lattice parameter (see Supplementary Fig. 2). By utilizing commensuration conditions, we identified the superstructure in the region **(I)** as a \(2\sqrt{3}\times 2\sqrt{3}\) arrangement, which has a twist angle of 30^{∘}, a Moiré angle of 30^{∘}, a supercell period of 1.23 nm, and a MoTe_{2} lattice constant of 3.55 Å (hereafter \(2\sqrt{3}\)R30^{∘} in Wood’s notation). In region **(III)**, we found the supercell to display a different structure, namely \(2\sqrt{7}\times 2\sqrt{7}\) with twist angle of 34.3^{∘}, a Moiré angle of 19.1^{∘}, a supercell period of 1.85 nm, and a MoTe_{2} lattice constant of 3.51 Å (hereafter \(2\sqrt{7}\)R19.1^{∘}). As the lattice constant of MoTe_{2} was reported previously to be 3.52 Å^{47}, our calculations show slight variations compared to this (~+0.8% and~−0.28%) in the different regions. Such a slight change in the lattice parameter (<1%) however is easily accommodated by van der Waals layers, as the commensuration can compensate for the excess elastic energy. We note that strain in this range (<1%) does not have a significant effect on the intrinsic electronic properties of MoTe_{2}. We also confirmed the resulting commensurate structures from the direct analysis of FFT images using the technique described in ref. ^{48} (see Supplementary Fig. 3). The superlattice corresponding to the found commensurate structures and the MoTe_{2} lattice line up remarkably well in the FFT images (see Supplementary Fig. 4), indicating indeed the commensurate nature of the Moiré domains.

The two Moiré patterns are linked across a grain boundary between domains **(I)** and **(III)** as marked in Fig. 2a, which separates the two different surface structures, indicating that there are more than one crystallographic orientation formed in the 1*H*-MoTe_{2} layer. As mentioned earlier, the LEED pattern suggests that these domains are randomly oriented. We emphasize here that the large size of the domain of the graphene grown on SiC almost excludes that this boundary is associated with the substrate. We extracted separate images of the two Moiré patterns corresponding to regions **(I)** and **(III)** from Fig. 2a, b, which are shown in Fig. 3. By applying fast Fourier transform (FFT) on these images (Fig. 3b, f for \(2\sqrt{3}\)R30^{∘} and Fig. 3d, h for \(2\sqrt{7}\)R19.1^{∘}), further details about the Moiré patterns can be revealed. The Fourier components appearing as bright spots in the FFT can be directly matched to the supercell units marked with color vectors in the real space STM images. In order to precisely determine these components, we measured the FFT intensity by using the k-space profiles for the \(2\sqrt{3}\)R30^{∘} and \(2\sqrt{7}\) R19.1^{∘} structures shown in Supplementary Fig. 5. We found that besides the periodic supercell of 1.23 and 1.85 nm, both Moiré patterns display an additional Fourier overtone corresponding to a periodicity of 0.7 nm. This component is a \(\sqrt{3}\) overtone of the \(2\sqrt{3}\) R30^{∘} supercell and a \(\sqrt{7}\) overtone of the \(2\sqrt{7}\) R19.1^{∘} supercell both having the same 2R0^{∘} Wood’s notation. For the sake of clarity hereinafter these structures are referred to as 2R0^{∘} and 2R’0^{∘}, respectively. With the help of Moiré theory, we will demonstrate later that these overtones incidentally coincide with the (2 × 2) lattice of the MoTe_{2} in both cases. This is also evident in the FFT image of Fig. 3h, where the (2 × 2) peaks align perfectly with the (1 × 1) lattice (see also Supplementary Fig. 4, where we show in Fourier-space that the superlattice lines up very well with the MoTe_{2} lattice, implying the commensurate property of the heterostructure). Moreover, the first (fundamental frequency) and second harmonics of the \(2\sqrt{7}\)R19.1^{∘} are also visible. The observed FFT components illustrated with various hexagons are shown in Fig. 3i. The most fascinating aspect in this FFT analysis of our STM results is that the bias voltage influences dramatically the distribution of the Fourier intensities among the many Moiré overtones. For example in the case of the \(2\sqrt{3}\)R30^{∘} structure, only the fundamental wavelength of 1.23 nm is observed at 1 V (Fig. 3f) while the second harmonic and \(\sqrt{3}\) overtone become visible with higher intensity at a lower bias voltage of 0.5 V (Fig. 3b). It also occurs similarly in the \(2\sqrt{7}\)R19.1^{∘} structure where the FFT intensity of the \(\sqrt{3}\) overtone (Fig. 3d orange hexagon) appears very strong at 0.5 V besides the first and second harmonics, while the \(\sqrt{7}\) overtone (Fig. 3h red hexagon) is prominent at 1 V rather than the \(\sqrt{3}\) one. The appearance of different overtones and harmonics depending on the bias voltage makes the STM image of such Moiré patterns highly variable.

The same analysis can be performed at the boundary of regions **(II)** and **(III)** as shown in Fig. 4a–c. Based on our STM images, we analyzed the Moiré structure in region **(II)** and we measured the Moiré periodicity to be about ~2.2 nm (Fig. 4d). Based on this, we identified the corresponding commensurate supercell (blue rhombus) to be a (\(\sqrt{39}\times \sqrt{39}\)) structure, having a twist angle of 33.1^{∘}, a Moiré angle of 16.1^{∘}, a 2.18 nm periodicity, and a MoTe_{2} lattice parameter of 3.50 Å (hereafter \(\sqrt{39}\)R16.1^{∘}) (see also Supplementary Fig. 3c). The apparent morphology of the supercell in the STM image consists of two triangles with bright spots surrounding a void located at the center as circled (marked by dark blue circles). The distance along a side of the triangle is nearly three times the lattice constant of 1*H*-MoTe_{2} and is illustrated in Fig. 4f. Model lattices of 1*H*-MoTe_{2} and graphene are constructed with a twist angle of about 33.1^{∘}, showing a match with the STM image. More details of the observed Moiré pattern of \(\sqrt{39}\)R16.1^{∘} are apparent in its corresponding FFT image in Fig. 4e. This pattern has an even richer Fourier spectrum compared to the previous ones. Not only the second (~1.1 nm) and third harmonics (~0.74 nm) of the fundamental frequencies of the supercell can be detected, but further Moiré overtones like \(\sqrt{7}\) (~0.85 nm) and even a \(\sqrt{13}\) (~0.63 nm) are visible. Indeed, we highlighted here such identified Fourier components of Fig. 4e in Fig. 4g with corresponding hexagons. Compared to Fig. 2, the similar behavior of the STM image taken on regions **(II)** and **(III)** with increasing the bias voltage (Fig. 4a–c) confirms the high variability of the measured real space Moiré patterns as a result of significant intensity changes in the Moiré overtones. Further details of FFT characterization for the Moiré patterns found in our system on other STM images are also provided in Supplementary Figs. 3, 4, 6, 7, 8.

### Moiré theory and DFT calculations of higher-indexed patterns

The Moiré patterns detected in our STM images have an unusually high degree of complexity compared to ones reported on other heterostructures in the literature. To reveal their nature, we analyzed the patterns in the context of Moiré theory found in refs. ^{30,32}. The possible Fourier components (\({\overrightarrow{K}}_{mnpq}\)) of the pattern are determined by the difference of the reciprocal lattices of the constituent layers, namely \({\overrightarrow{K}}_{mnpq}={\overrightarrow{G}}_{pq}^{\prime}-{\overrightarrow{G}}_{mn}\), where \({\overrightarrow{G}}_{mn}\) is a reciprocal lattice vector of the graphene and \({\overrightarrow{G}}_{pq}^{\prime}\) is a reciprocal lattice vector of the MoTe_{2} lattice. During rotation of the layers whenever any \({\overrightarrow{G}}_{pq}^{\prime}\) and \({\overrightarrow{G}}_{mn}\) vectors get close to each other in reciprocal space, a Moiré pattern emerges in real space with a wavelength of \({\lambda }_{mnpq}=2\pi /| {\overrightarrow{K}}_{mnpq}|\). Based on this, we denote Moiré patterns with these four indices (*m**n**p**q*), which define a unit cell vector in the k-space of this particular pattern. In this paper, we used an acute coordinate system, when defining the actual (*m**n**p**q*) indices, so that the unit cell vectors of the atomic lattices form 60^{∘} angle in reciprocal space (for details see Supplementary Fig. 9). In the case of simple geometrical lattices, the Moiré pattern, perceived by our eyes, arises from the lattices modulating the intensity of the visible light passing through them. In such an optical scenario, the larger the indices, the smaller the Fourier amplitudes following a heavily decreasing relationship^{30}. Such optical analogy turned out to be very well applicable to atomic lattices to describe the Fourier spectrum of Moiré patterns measured by STM^{31}. On this basis, the most common Moiré pattern formed between hexagonal lattices is the one with the lowest possible (*m**n**p**q*) indices i.e., (1010) with a maximum wavelength at 0^{∘} twist angle, which was indeed found in the vast majority of cases^{39,49,50,51,52,53,54}, while patterns with higher indices were identified in a few occasions only (graphene/Ir(111)^{36}, graphene/Al(111)^{37}, and graphene/ReS_{2}^{55}). We assume that this is partly because their potential modulation is weak and therefore can not easily be detected by STM measurements.

In order to elaborate on higher-indexed Moire patterns in the context of the present study, we numerically calculated the *λ*_{mnpq} wavelength of some indices for the entire twist angle spectrum (*θ* = 0^{∘} − 60^{∘}) of the MoTe_{2}/graphene heterostructure for a small range of MoTe_{2} lattice parameters around the reported value of 3.52 Å (Fig. 5a). It is immediately noticeable that the wavelength of the (1010) pattern stays well below the experimentally measured Moiré periodicities of 1.23, 1.85, and 2.2 nm (see purple curves of Fig. 5a) and around 30^{∘} its wavelength becomes comparable to the atomic lattice of the MoTe_{2} surface layer. Then it will no longer be observable. The invisible (1010) pattern around 30^{∘} provides an opportunity for other patterns to become observable as they do not overlap in real space with the dominant Moiré anymore. The (1110) pattern for example, with a wavelength peak at the twist angle of 30^{∘} (see yellow curves of Fig. 5a) is the second visually most prominent pattern after (1010). Therefore, it immediately becomes visible to the eye in real space as we rotated a model of atomic lattices on top of each other to form the \(2\sqrt{3}\)R30^{∘}, \(2\sqrt{7}\)R19.1^{∘}, and \(\sqrt{39}\)R16.1^{∘} superstructures (see red rhombus in Fig. 5b) and yellow rhombuses in Fig. 5c, d). The (1110) pattern apparent in Fig. 5b can be directly matched with the experimental Moiré pattern, in particular with the \(2\sqrt{3}\)R30^{∘} structure previously shown in Fig. 3e both having the same 1.23 nm period. However, the further experimental values of 1.85 and 2.2 nm exceed the maximum wavelength of the (1110) pattern, indicating additional mechanisms to be revealed. Specifically, it can be shown that these larger periods equal the length of commensurate supercells of the \(2\sqrt{7}\)R19.1^{∘} and \(\sqrt{39}\)R16.1^{∘} structures. Commensuration in real space implies that a supercell can be defined besides the usual Moiré patterns. This supercell, in contrast to Moiré patterns in general, possesses perfect atomic periodicity, which happens only for particular discrete twist angles and lattice mismatches^{45}. In Fig. 5b–d, we displayed these commensurate supercells with red rhombuses.

As can be seen from these images, the supercells fit the (1110) pattern in different ways. In the case of \(2\sqrt{3}\)R30^{∘}, the supercell is equivalent to the (1110) Moiré: (1 × 1)*λ*_{1110} (see Fig. 5b), while for \(2\sqrt{7}\)R19.1^{∘} we have \((\sqrt{3}\times \sqrt{3}){\lambda }_{1110}\) (see Fig. 5c) and a (2 × 2)*λ*_{1110} structure in the case of \(\sqrt{39}\)R16.1^{∘} (see Fig. 5d). The supercells represent an extra modulation in the (1110) pattern that becomes visible on the STM images. Indeed, the Moiré beatings differ slightly on the atomic scale and only become perfectly identical with the period of the supercell in the (1110) pattern for the \(2\sqrt{7}\)R19.1^{∘} and \(\sqrt{39}\)R16.1^{∘} structures (corners of the red rhombuses in Fig. 5c, d). Only perfectly identical beatings will have the same STM contrast, therefore highlighting the supercell periods. The strong appearance of the supercell periods suggests that STM images of the MoTe_{2}/graphene system have a high sensitivity to the electronic properties in which the small atomic deviations of the Moiré stackings result in significant differences in the tunneling current. This will be further analysed in our DFT calculations below. Therefore, the (1110) pattern with the commensurate supercell periods displayed in Fig. 5b–d describe quantitatively the experimental patterns shown in Figs. 3e, g, 4d. Moreover, the commensurate supercells can be interpreted in Moiré theory as even higher-indexed Moiré patterns. To highlight this, we indicated the experimentally measured Moiré periods with blue stars in Fig. 5a. The measured Moiré periods sit very well on a calculated higher-indexed \({\lambda }_{313\overline{1}}\) curve, which has a maximum wavelength of 2.28 nm at *θ* = 33^{∘} twist angle (see the red curve of Fig. 5a) supporting the higher-indexed origin of the experimental patterns.

The concept of the higher-indexed patterns and supercells is further verified by calculating the \({\overrightarrow{K}}_{mnpq}\) Moiré reciprocal vectors of the abovementioned commensurate supercells. We plotted them for each measured structure (Fig. 6a–c blue dots). In the figure, the smaller the indices of a \({\overrightarrow{K}}_{mnpq}\) component have, the bigger the blue dot we choose. It can be seen that the experimentally detected Fourier components in Figs. 3, 4 are fully reproduced by this method. We note that among the calculated Fourier components, the atomic lattice and the (1010) pattern (blue and dotted hexagons) are also highlighted, which are usually absent in the FFT images of the measurement. The fundamental frequencies correspond to the supercell periods of 1.23 nm (Fig. 6a), 1.85 nm (Fig. 6b), and 2.18 nm (Fig. 6c) are in perfect agreement with the experimentally measured periodicities. As can be seen, the dots depicting the fundamental frequencies are small compared to other points on the spectrum, which means that these patterns have high indices, namely the (313\(\overline{1}\)) mentioned earlier. The additional Moiré overtones detected in the measurements as patterns with smaller wavelengths (~0.7 nm) such as 2R0^{∘} (*θ* = 30^{∘}) and 2R’0^{∘} (*θ* = 34.3^{∘}) structures are also fully reproduced (see red hexagons in Fig. 6a, b), among the other experimental overtones of the \(\sqrt{39}\)R16.1^{∘} structure (Fig. 6c). Figure 6a–c show the possible Fourier components of the investigated geometries with the corresponding Moiré indices in Fig. 6d. The complex electronic properties of the system define which Fourier component will be appeared in the STM image at different voltages among the many possible Moiré overtones. Based on the overtones, we found that the smaller Moiré periods such as 2R0^{∘}(*θ* = 30^{∘}) (detected under lower bias voltage in Fig. 3b) and 2R’0^{∘} (*θ* = 34.3^{∘}) (detected at higher bias voltage in Fig. 3h) correspond to the (0211) higher indices (see red hexagons in Fig. 6d and the green theoretical *λ*_{0211} curve in Fig. 5a). Therefore, we conclude that the variation of the bias voltage transforms the Moiré pattern from (313\(\overline{1}\)) to (0211).

In order to investigate the connection between higher-indexed Moiré patterns and the electronic properties, we performed DFT electronic structure calculations taking into account the vdW interaction effects. For the calculations, we choose the 2\(\sqrt{3}\)R30^{∘} geometry which has the smallest supercell size among the experimentally observed structures. The geometry relaxation revealed negligible corrugation effects, therefore both the graphene and the MoTe_{2} layers remain flat at 30^{∘} rotation angle similar to the case of the previously investigated MoS_{2}/graphene heterostructure^{56}. The absence of the atomic corrugation highlights the electronic structure origin of the observed Moiré patterns. The calculated total density of states (DOS) and also the sum of the partial DOS of the different atoms (C, Te, Mo) in the supercell are presented in Fig. 7a. The Fermi level is situated in the bandgap of the MoTe_{2} (~1 eV), where no additional gap states are formed. We note that in the DFT calculations the Fermi level coincides with the Dirac point of the graphene (see Supplementary Fig. 10), while in the measurements the graphene is strongly n-doped (E_{D} ~ −0.4 eV) due to the SiC(0001) substrate (see Supplementary Fig. 11), rendering the Fermi level close to the conduction band minimum (CBM) of the MoTe_{2}. Therefore, substrate-induced doping should be considered when comparing the simulated and measured STM images at a given bias voltage.

Figure 7c–e show the calculated dI/dV maps at *z* = 5 Å tip-sample distance for +0.7, +1.0, and +1.8 V bias values in the area marked in Fig. 7a. We found significant differences on these maps originating from the highly variable spatial distributions of the charge density due to the complex electronic structure of the system. The maximum dI/dV values at different bias voltages are located in some cases on the Mo atoms (*V* = 0.7 V), in other cases on the Te atoms (*V* = 1.0 V), and even they can be situated on the center of MoTe_{2} hexagons (*V* = 1.8 V). However, we revealed that this property is intrinsic to the single-layer MoTe_{2}, irrespective of the graphene substrate. As can be seen from Fig. 7a, at +0.7 eV only Mo atoms have finite DOS values resulting in maxima on the Mo atoms in the corresponding simulated dI/dV map (Fig. 7c). By contrast, the Te atoms appear much brighter in the dI/dV map at +1.0 V (Fig. 7d), despite the fact that the Mo atoms still present higher DOS values. This means that the geometrical effect arising from the height difference of the Mo and Te atomic planes, i.e., the Te atoms are located at 1.8 Å higher than the Mo atoms, compensates for the larger Mo contribution to the DOS. We observed further contrast change at an increased bias value (+1.8 V), where the dI/dV maxima are localized at the center of the MoTe_{2} hexagons (Fig. 7e). This spatial distribution originates from the increased weight of the in-plane *p*_{x}, *p*_{y} orbitals of Te and *d*_{xz}, *d*_{yz} orbitals of Mo atoms (see Supplementary Fig. 12). Besides the varying location of the dI/dV maximum with the bias voltage intrinsic to the MoTe_{2} layer, the dI/dV values are further perturbed by the electronic interactions mediated between the graphene substrate and the MoTe_{2} resulting that the same type of atoms are not equivalent inside the supercell. This is further illustrated by the inhomogeneous electronic density redistribution^{57} resulting from the charge transfer between the graphene and MoTe_{2} layers (see Supplementary Fig. 13). In detail, our DFT calculations indicate the accumulation of localized electrons on the bottom Te layer atoms while the depletion of delocalized electrons occurs from the graphene layer. This localized nature of the charge transfer causes spatial sensitivity because the relative positions between the carbon and Te atoms play a more important role. This sensitivity to small deviances in atomic positions is crucial for higher-indexed patterns to become visible in STM measurements. In accordance with this, it can be seen that even small changes in the local environment of the Mo and Te atoms in the supercell can result in significantly different dI/dV maxima along the corresponding Moiré periods, for example, those Te atoms have dI/dV maximum in Fig. 7d, which are situated on top of C-C bonds. This implies the important effect of the otherwise weak Moiré potential modulations. From the simulated dI/dV maps, we can conclude that the competing contributions to the DOS from the Mo and Te atoms together with the effect of the underlying graphene substrate lead to various patterns in the dI/dV maps at different bias voltages, explaining the sensitivity of the STM images in the measurements.

More importantly, simulated surface topographies (STM images) confirm the existence of higher-indexed patterns with different periodicities (see Fig. 7f–h). Due to substrate doping effects, the first dominant DOS peak of the CBM is situated at +0.2 V in the STS measurement. However, this DOS peak is located at +1 V in our DFT calculations, where the doping effect of the SiC substrate is neglected. Therefore, the +1.0 and +1.8 V bias voltages used in the simulated STM images (Fig. 7g, h) correspond to roughly +0.2 and +1.0 V in the experiments (Fig. 2c, a). We note, that this correspondence can only be approximate, due to the differences in the fine details between the theoretical and experimental band structures. For example, the SiC substrate doping is not rigidly shifting the bandstructure, as it is unevenly distributed between the layers of the heterostructure. From our DFT calculations, we found that the commensurate supercell dominates in the simulated STM image at a larger tip-bias voltage (+1.8 V) (Fig. 7h), where the center of the MoTe_{2} hexagons at the supercell corners are visible. This pattern is equivalent to the *λ*_{1110} Moiré pattern with a 1.23 nm wavelength in perfect agreement with the experimentally observed periodicity in the measured STM image in Fig. 3e. For comparison, we have shown again side by side the measured and simulated STM images in Supplementary Fig. 12. At lower voltage (+1 V) in the simulation (Fig. 7g), second neighbor Te atoms appear as protrusions and their center as depression resulting in an additional 0.7 nm periodicity in the simulated STM image besides the supercell periodicity. This 0.7 nm periodicity is equal to the \(\sqrt{3}\) overtone (*λ*_{0211}), which is also detected in the measured STM image at the corresponding voltage in Fig. 2c. As the higher-indexed *λ*_{0211} tends to have a weaker potential modulation, it is more prone to be perturbed by weak substrate effects such as the presence of the SiC, which is neglected in our simulations. This may contribute to the small differences found between the simulated STM image and the measurements in this case. Nevertheless, our simulated STM images clearly show the change of the Fourier intensities and the appearance of different simultaneous Moiré periods with the bias voltage, while presenting a great variety of patterns, which we have already seen in the STM experiments.

Finally, based on our findings we address the question of the presence of higher-indexed Moiré patterns in other vdW heterostructures. As we have shown several conditions have to be fulfilled for the higher-indexed Moiré patterns to be visible in STM. Namely, (I) the twist angle between the hexagonal lattices should be around 30^{∘}, (II) the wavelength of higher-indexed Moiré patterns has to be in the measurable range (i.e., of the order of the nm), and (III) the weak potential modulations of the higher-indexed Moiré have to lead to changes of the electronic properties of the heterostructure with measurable STM fingerprints. Condition II constrains the lattice parameter of the constituent lattices. Based on these criteria higher-indexed Moiré patterns might have a chance to be observable in other heterostructures such as those based on graphene with other TMDs. Indeed, TMD lattice parameters are similar to MoTe_{2} one (~3.1−3.5 Å), which makes the wavelength of higher-indexed Moiré patterns to be in the measurable range. Their electronic properties also show similarities including the orbital contributions of the transition metal and the chalcogen atoms. We note that the Moiré pattern observed on graphite/MoS_{2} heterostructures around 27^{∘} twist angle^{58} is probably the signature of a higher-indexed Moiré. However, the main importance of the higher-indexed Moiré patterns lies in the fact that Moiré physics can also occur in many other heterostructures, which has not been considered previously in the field of twistronics. For example, recent measurements^{59} show that higher-indexed Moiré patterns in graphene/xenon heterostructures effectively tailor the Dirac fermions, similar to the case of twisted bilayer graphene.

In conclusion, we investigated the formation of a variety of Moiré structures in 1*H*-MoTe_{2} films on graphene terminated 6*H*-SiC(0001) under appropriate MBE growth conditions by STM. Three different patterns (\(2\sqrt{3}\)R30^{∘}, \(\sqrt{39}\)R16.1^{∘}, and \(2\sqrt{7}\)R19.1^{∘}) were observed using various tunneling conditions. They exhibit unusually rich and complex Moiré structures with the appearance of higher-indexed Moiré patterns predicted by Moiré theory. Additional Moiré overtones appeared in the measurements, which predominated in the pattern at certain voltages, making the electronic Moiré highly variable with the bias in the real space STM images. Our results also show a strong signature in the STM images of commensurate supercells around 30^{∘}, which are very faint in most heterostructures. DFT calculations and STM simulations have explained the complex Moiré patterns by revealing the importance of the electronic coupling between the layers in the MoTe_{2}/graphene heterostructure even for weaker Moiré potential modulations. Due to the important role that Moiré patterns already play in twistronics phenomena, we believe that higher-indexed patterns can further expand the possibilities of Moiré physics in the field of vdW heterostructures.

## Methods

### Sample preparation

In this study, graphene on n-type doped 6*H*-SiC(0001) was used as a substrate for the growth of MoTe_{2} films. Following a vacuum graphitization process of 6*H*-SiC(0001) as detailed by ref. ^{60}, large-scale uniform double-layer graphene with the root mean square surface roughness of ~0.1–0.2 nm was obtained. The high crystalline quality of single-layer 2*H*-MoTe_{2} films was formed on top of graphene by a multi-step MBE process as reported in our previous work^{9}. After the 2*H*-MoTe_{2} formation, a sample was taken out of the MBE chamber and preserved in a clean dry box filled with nitrogen gas from a pressurized nitrogen gas cylinder (≥99.9% pure) to avoid oxygen contamination as much as possible due to air exposure during transportation^{61}.

### STM characterization

Samples were transferred to low-temperature STM (Omicron) working at ~5 K and at a pressure lower than 1 × 10^{−11} mbar. Before STM imaging, the sample was outgassed around ~250 ^{∘}C for 10 min to clean its surface. The STM topographic images were taken at constant current mode using an electro-chemically etched tungsten tip.

### Computational details

Electronic structure calculations were performed in the framework of DFT implemented in the Vienna ab initio simulation package (VASP)^{62} using the plane-wave basis set and projector augmented wave method^{63}. The rev-vdW-DF2 functional was used to include properly the vdW interaction^{64,65}. The hexagonal supercell of the MoTe_{2}/graphene heterostructure (\(2\sqrt{3}\)R30^{∘}) has a supercell period of *a* = 12.23 Å and contains 24 Te, 12 Mo, and 50 C atoms, respectively. Atomic positions were relaxed using the conjugate-gradient method until the forces of the atoms were reduced to 0.01 eV/Å and the cut-off energy for the plane-wave basis set was chosen to be 500 eV. To avoid artificial interactions between periodic replicas of the MoTe_{2}/graphene layers, a vacuum interval of 18 Å was introduced in the *z*-direction. The Brillouin zone was sampled with (5 × 5 × 1) Monkhorst–Pack mesh^{66} for geometry optimization, and (30 × 30 × 1) for density-of-states calculations. Simulated STM images were obtained by using the Tersoff-Hamann approximation^{67} implemented as an *s*-type tip in the revised Chen method^{68} in the BSKAN code^{69,70}.

## Data availability

The authors confirm that the data supporting the findings of this study are available within the article and the Supplementary Materials. Related additional data were available on reasonable request from the authors.

## References

Choi, W. et al. Recent development of two-dimensional transition metal dichalcogenides and their applications.

*Mater. Today***20**, 116–130 (2017).Gutierrez, H. R. et al. Extraordinary room-temperature photoluminescence in triangular WS

_{2}monolayers.*Nano Lett.***13**, 3447–3454 (2013).Pei, J. J., Yang, J., Yildirim, T., Zhang, H. & Lu, Y. R. Many-body complexes in 2D semiconductors.

*Adv. Mater.***31**, 1706945 (2019).Tsai, M. L. et al. Monolayer MoS

_{2}heterojunction solar cells.*ACS Nano***8**, 8317–8322 (2014).Mu, C., Xiang, J. & Liu, Z. Photodetectors based on sensitized two-dimensional transition metal dichalcogenides-A review.

*J. Mater. Res.***32**, 4115–4131 (2017).Wang, C., Yang, F. & Gao, Y. The highly-efficient light-emitting diodes based on transition metal dichalcogenides: from architecture to performance.

*Nanoscale Adv.***2**, 4323–4340 (2020).Lee, H., Ahn, J., Im, S., Kim, J. & Choi, W. High-responsivity multilayer MoSe

_{2}phototransistors with fast response time.*Sci. Rep.***8**, 11545 (2018).Song, S. et al. Room temperature semiconductor-metal transition of MoTe

_{2}thin films engineered by strain.*Nano Lett.***16**, 188–193 (2016).Pham, T. T., Castelino, R., Felten, A. & Sporken, R. Preparation of single phase 2H-MoTe

_{2}films by molecular beam epitaxy.*Appl. Surf. Sci.***523**, 146428 (2020).Zhou, L. et al. Large-area synthesis of high-quality uniform few-layer MoTe

_{2}.*J. Am. Chem. Soc.***137**, 11892–11895 (2015).Keum, D. H. et al. Bandgap opening in few-layered monoclinic MoTe

_{2}.*Nat. Phys.***11**, 482–486 (2015).Yoo, Y., DeGregorio, Z. P., Su, Y., Koester, S. J. & Johns, J. E. In-plane 2H-1T’ MoTe

_{2}homojunctions synthesized by flux-controlled phase engineering.*Adv. Mater.***29**, 1605461 (2017).Conan, A., Bonnet, A., Amrouche, A. & Spiesser, M. Semiconducting properties and band structure of MoTe

_{2}single crystals.*J. Phys.***45**, 459–465 (1984).Sankar, R. et al. Polymorphic layered MoTe

_{2}from semiconductor, topological insulator, to Weyl semimetal.*Chem. Mater.***29**, 699–707 (2017).Rhodes, D. et al. Engineering the structural and electronic phases of MoTe

_{2}through W substitution.*Nano Lett.***17**, 1616–1622 (2017).Zhou, J. et al. Large-area and high-quality 2D transition metal telluride.

*Adv. Mater.***29**, 1603471 (2017).Empante, T. A. et al. Chemical vapor deposition growth of few-layer MoTe

_{2}in the 2H, 1T’, and 1T phases: tunable properties of MoTe_{2}films.*ACS Nano***11**, 900–905 (2017).Zhou, L. et al. Synthesis of high-quality large-area homogenous 1T’-MoTe

_{2}from chemical vapor deposition.*Adv. Mater.***28**, 9526–9531 (2016).Shi, D., Wang, G., Li, C., Shen, X. & Nie, Q. Preparation and thermoelectric properties of MoTe

_{2}thin films by magnetron co-sputtering.*Vacuum***138**, 101–104 (2017).Vishwanath, S. et al. MBE growth of few-layer 2H-MoTe

_{2}on 3D substrates.*J. Cryst. Growth***482**, 61–69 (2018).Yu, Y. et al. Molecular beam epitaxy growth of atomically ultrathin MoTe

_{2}lateral heterophase homojunctions on graphene substrates.*Carbon***115**, 526–531 (2017).Yu, Y. et al. Phase-controlled growth of one-dimensional Mo

_{6}Te_{6}nanowires and two-dimensional MoTe_{2}ultrathin films heterostructures.*Nano Lett.***18**, 675–681 (2018).Tang, S. et al. Electronic structure of monolayer 1T’-MoTe

_{2}grown by molecular beam epitaxy.*APL Mater.***6**, 026601 (2018).Zhang, C. et al. Charge mediated reversible metal-insulator transition in monolayer MoTe

_{2}and W_{x}Mo_{1-x}Te_{2}alloy.*ACS Nano***10**, 7370–7375 (2016).Castelino, R., Pham, T. T., Felten, A. & Sporken, R. Substrate temperature dependence of the crystalline quality for the synthesis of pure-phase MoTe

_{2}on graphene/6H-SiC(0001) by molecular beam epitaxy.*Nanotechnology***31**, 115702 (2019).Diaz, H. C. et al. Substrate dependent electronic structure variations of van der Waals heterostructures of MoSe

_{2}or MoSe_{2}(1-x) Te2x grown by van der Waals epitaxy.*2D Mater.***4**, 025094 (2017).Hermann, K. Periodic overlayers and moiré patterns: theoretical studies of geometric properties.

*J. Phys. Condens. Matter***24**, 314210 (2012).Gadelha, A. C. et al. Localization of lattice dynamics in low-angle twisted bilayer graphene.

*Nature***590**, 405–409 (2021).Cao, Y. et al. Unconventional superconductivity in magic-angle graphene superlattices.

*Nature***556**, 43–50 (2018).Zeller, P. & Günther, S. What are the possible moiré patterns of graphene on hexagonally packed surfaces? Universal solution for hexagonal coincidence lattices, derived by a geometric construction.

*New J. Phys.***16**, 083028 (2014).Zeller, P., Ma, X. & Günther, S. Indexing moiré patterns of metal-supported graphene and related systems: strategies and pitfalls.

*New J. Phys.***19**, 013015 (2017).Le Ster, M., Markl, T. & Brown, S. Moiré patterns: a simple analytical model.

*2D Mater.***7**, 011005 (2019).Bistritzer, R. & MacDonald, A. H. Moiré bands in twisted double-layer graphene.

*Proc. Natl Acad. Sci. USA***108**, 12233–12237 (2011).Yankowitz, M., Xue, J. & LeRoy, B. J. Graphene on hexagonal boron nitride.

*J. Phys. Condens. Matter***26**, 303201 (2014).Diaz, H. C., Chaghi, R., Ma, Y. & Batzill, M. Molecular beam epitaxy of the van der Waals heterostructure MoTe

_{2}on MoS_{2}: phase, thermal, and chemical stability.*2D Mater.***2**, 044010 (2015).Loginova, E., Nie, S., Thurmer, K., Bartelt, N. C. & McCarty, K. F. Defects of graphene on Ir(111): rotational domains and ridges.

*Phys. Rev. B***80**, 085430 (2009).Zhang, S., He, D., Huang, P. & Wang, F. Moiré pattern at graphene/Al (111) interface: experiment and simulation.

*Mater. Des.***201**, 109509 (2021).Szendrő, M., Pálinkás, A., Sule, P. & Osváth, Z. Anisotropic strain effects in small-twist-angle graphene on graphite.

*Phys. Rev. B***100**, 125404 (2019).Voloshina, E. N. et al. Electronic structure and imaging contrast of graphene Moiré on metals.

*Sci. Rep.***3**, 1072 (2013).Liu, H. et al. Dense network of one-dimensional midgap metallic modes in monolayer MoSe

_{2}and their spatial undulations.*Phys. Rev. Lett.***113**, 066105 (2014).Diaz, H. C., Ma, Y., Chaghi, R. & Batzill, M. High density of (pseudo) periodic twin-grain boundaries in molecular beam epitaxy-grown van der Waals heterostructure: MoTe

_{2}/MoS_{2}.*Appl. Phys. Lett.***108**, 191606 (2016).Ma, Y. et al. Metallic twin grain boundaries embedded in MoSe

_{2}monolayers grown by molecular beam epitaxy.*ACS Nano***11**, 5130–5139 (2017).Coelho, P. M. et al. Post-synthesis modifications of two-dimensional MoSe

_{2}or MoTe_{2}by incorporation of excess metal atoms into the crystal structure.*ACS Nano***12**, 3975–3984 (2018).Wang, L. et al. Direct observation of one-dimensional peierls-type charge density wave in twin boundaries of monolayer MoTe

_{2}.*ACS Nano***14**, 8299–8306 (2020).Merino, P., Svec, M., Pinardi, A. L., Otero, G. & Martin-Gago, J. A. Strain-driven Moiré superstructures of epitaxial graphene on transition metal surfaces.

*ACS Nano***5**, 5627–5634 (2011).Meng, L. et al. Multi-oriented moiré superstructures of graphene on Ir(111): experimental observations and theoretical models.

*J. Phys. Condens. Matter***24**, 314214 (2012).Dawson, W. G. & Bullett, D. W. Electronic structure and crystallography of MoTe

_{2}and WTe_{2}.*J. Phys. C. Solid State Phys.***20**, 6159 (1987).Günther, S., Zeller, P., Böller, B. & Wintterlin, J. Method for the manual analysis of Moiré structures in STM images.

*ChemPhysChem***22**, 870–884 (2021).Sule, P., Szendrő, M., Magda, G. Z., Hwang, C. & Tapaszto, L. Nanomesh-type graphene superlattice on Au (111) substrate.

*Nano Lett.***15**, 8295–8299 (2015).Wang, B., Bocquet, M.-L., Marchini, S., Günther, S. & Wintterlin, J. Chemical origin of a graphene moiré overlayer on Ru(0001).

*Phys. Chem. Chem. Phys.***10**, 3530–3534 (2008).Woods, C. et al. Commensurate-incommensurate transition for graphene on hexagonal boron nitride.

*Nat. Phys.***10**, 451–456 (2014).Koos, A. A. et al. Influence of native defects on the electronic and magnetic properties of CVD grown MoSe

_{2}single layers.*J. Phys. Chem. C***123**, 24855–24864 (2019).Krane, N., Lotze, C. & Franke, K. J. Moiré structure of MoS

_{2}on Au (111): local structural and electronic properties.*Surf. Sci.***678**, 136–142 (2018).Geng, W., Wang, V., Liu, Y., Ohno, T. & Nara, J. Moiré potential, lattice corrugation, and band gap spatial variation in a twist-free MoTe

_{2}/MoS_{2}heterobilayer.*J. Phys. Chem. Lett.***11**, 2637–2646 (2020).Plumadore, R., Al Ezzi, M. M., Adam, S. & Luican-Mayer, A. Moiré patterns in graphene-rhenium disulfide vertical heterostructures.

*J. Appl. Phys.***128**, 044303 (2020).Di Felice, D., Abad, E., Gonzalez, C., Smogunov, A. & Dappe, Y. Angle dependence of the local electronic properties of the graphene/MoS

_{2}interface determined by ab initio calculations.*J. Phys. D Appl. Phys.***50**, 17LT02 (2017).Wang, B., Günther, S., Wintterlin, J. & Bocquet, M.-L. Periodicity, work function and reactivity of graphene on Ru(0001) from first principles.

*New J. Phys.***12**, 043041 (2010).Trainer, D. J. et al. Moiré superlattices and 2D electronic properties of graphite/MoS2 heterostructures.

*J. Phys. Chem. Solids***128**, 325–330 (2019).Wu, C. et al. Tailoring Dirac fermions by in-situ tunable high-order moiré pattern in graphene-monolayer xenon heterostructure. Preprint at http://arXiv.org/abs/2203.09705 (2022).

Wang, Q. et al. Large-scale uniform bilayer graphene prepared by vacuum graphitization of 6H-SiC(0001) substrates.

*J. Phys. Condens. Matter***25**, 095002 (2013).Pham, T. T., Castileno, R., Felten, A. & Sporken, R. Study of surface oxidation and recovery of clean MoTe

_{2}films.*Surf. Interfaces***28**, 101681 (2022).Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector augmented-wave method.

*Phys. Rev. B***59**, 1758 (1999).Blochl, P. E. Projector augmented-wave method.

*Phys. Rev. B***50**, 17953 (1994).Klimes, J., Bowler, D. R. & Michaelides, A. Van der Waals density functionals applied to solids.

*Phys. Rev. B***83**, 195131 (2011).Hamada, I. van der Waals density functional made accurate.

*Phys. Rev. B***89**, 121103 (2014).Monkhorst, H. J. & Pack, J. D. Special points for Brillouin-zone integrations.

*Phys. Rev. B***13**, 5188 (1976).Tersoff, J. & Hamann, D. Theory and application for the scanning tunneling microscope.

*Phys. Rev. Lett.***50**, 1998 (1983).Mandi, G. & Palotas, K. Chen’s derivative rule revisited: role of tip-orbital interference is STM.

*Phys. Rev. B***91**, 165406 (2015).Hofer, W. A. Challenges and errors: interpreting high resolution images in scanning tunneling microscopy.

*Prog. Surf. Sci.***71**, 147–183 (2003).Palotas, K. & Hofer, W. A. Multiple scattering in a vacuum barrier obtained from real-space wavefunctions.

*J. Phys. Condens. Matter***17**, 2705 (2005).

## Acknowledgements

We would like to thank Etienne Gennart and Jean-Pierre Van Roy for their technical support. Trung T. Pham would like to thank ARES CCD for financial support and Roshan Castelino acknowledges a scholarship from the Jesuit province of l’EOF. The work was supported by the European H2020 GrapheneCore3 Project No. 881603, Graphene Flagship, and the Élvonal grant KKP 138144. P.V. and K.P. acknowledge the support of the Janos Bolyai Research Scholarship of the Hungarian Academy of Sciences. M.S., K.P., and P.V. acknowledge the support from the National Research, Development and Innovation Office (NKFIH) in Hungary, through Grants No. K-134258, FK-124100, and K-132869. This research used resources of the “Plateforme Technologique de Calcul Intensif (PTCI)” located at the University of Namur, Belgium which is supported by the F.R.S.-FNRS under the convention No. 2.5020.11. The PTCI is member of the “Consortium des Équipements de Calcul Intensif (CÉCI)”. M.B., C.C., and J.L. acknowledge the European Union for funding (Grant Agreement No. 766726).

## Author information

### Authors and Affiliations

### Contributions

R.S. and T.T.P. conceived and designed the experiments. T.T.P. and R.C. prepared the samples. T.T.P., R.C., C.C., M.B., and J.L. performed the low-temperature STM measurements. T.T.P. analyzed the experimental data while P.V., M.S., and K.P. carried out the Moiré and DFT calculations. R.S. and L.H. supervised the project. T.T.P., M.S., and P.V. wrote the paper. All authors discussed the results and commented on the manuscript. T.T.P., P.V., and M.S. contributed equally to the work.

### Corresponding authors

## Ethics declarations

### Competing interests

The authors declare no competing interests.

## Additional information

**Publisher’s note** Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Supplementary information

## Rights and permissions

**Open Access** This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.

## About this article

### Cite this article

Pham, T.T., Vancsó, P., Szendrő, M. *et al.* Higher-indexed Moiré patterns and surface states of MoTe_{2}/graphene heterostructure grown by molecular beam epitaxy.
*npj 2D Mater Appl* **6**, 48 (2022). https://doi.org/10.1038/s41699-022-00321-9

Received:

Accepted:

Published:

DOI: https://doi.org/10.1038/s41699-022-00321-9